Standard Test Method for Determination of Water/Cementitious Materials Ratio for Geosynthetic Cementitious Composite Mats (GCCMs) and Measurement of the Compression Strength of the Cementitious Material Contained WithinTranslate name
STANDARD published on 1.6.2020
Designation standards: ASTM D8329-20
Publication date standards: 1.6.2020
The number of pages: 3
Approximate weight : 9 g (0.02 lbs)
Country: American technical standard
Category: Technical standards ASTM
compressive strength, GCCM, geosynthetic cementitious composite mat, water/cementitious material ratio,
|Significance and Use|
5.1 Hydration is a critical aspect of GCCM installation. GCCM installations are often hydrated with excess water to ensure that a saturated condition exists. Therefore, it is not generally possible to monitor and control exactly the water addition that absorbs and hydrates the cementitious materials due the practical methods of hydration in use.
5.2 It is important to be able to distinguish the quality of cementitious material used in applications for GCCMs. A measurement of compressive strength properties of the cementitious material is often an accepted method to provide a measure of the cement strength and quality. The compressive strength properties will vary with the water/cementitious material ratio and, therefore, it is necessary to determine a practical value that approximates in-use hydration and not a water/cementitious material ratio that simply provides the maximum properties but cannot be expected as representative of actual use conditions.
5.3 The compressive strength of the cementitious material can be affected by both over and under hydration.
5.4 This method identifies a means to obtain a water/cementitious material ratio representative of that obtained by proper hydration of GCCMs to allow replication for laboratory compressive strength testing for use by GCCM designers, inspectors, and installers.
1.1 The purpose of the proposed test method is to obtain a water/cementitious material ratio that allows for a practical measurement of the compressive strength of the cementitious material contained within a geosynthetic cementitious composite mat (GCCM). This water/cementitious material ratio should be generally representative of that achieved practically upon the hydration of a GCCM. Because GCCM materials do not involve mixing or the use of exact water hydration methods when employed in the field, this method is necessary to provide a quantitative estimate of the water/cementitious material ratio.
1.2 This procedure determines the water/cementitious material ratio for a properly hydrated GCCM, which is then used to create cube or cylinder specimens for compressive strength testing as per the appropriate referenced ASTM test methods. Compressive strength results will then be representative of the strength of the inherent cementitious material found in the GCCM after normal GCCM hydration.
1.3 The values in SI units are to be regarded as standard. Values in inch-pound units are in parentheses for information.
1.4 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety, health, and environmental practices and determine the applicability of regulatory limitations prior to use.
1.5 This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards, Guides and Recommendations issued by the World Trade Organization Technical Barriers to Trade (TBT) Committee.
Do you want to make sure you use only the valid technical standards?
We can offer you a solution which will provide you a monthly overview concerning the updating of standards which you use.
Would you like to know more? Look at this page.
Latest update: 2021-04-18 (Number of items: 2 441 221)
© Copyright 2021 NORMSERVIS s.r.o.